PHYSICAL REVIEW B 1 MARCH 1997-IIVOLUME 55, NUMBER 10Frequency upconversion in Er31-doped fluoroindate glasses pumped at 1.48mm
G. S. Maciel and Cid B. de AraujoDepartamento de Fsica, Universidade Federal de Pernambuco, 50670-901 Recife, PE, Brazil
Y. MessaddeqDepartamento de Qumica, Universidade do Estado de Sao Paulo, 14800-900 Araraquara, SP, Brazil
M. A. AegerterInstitut fur Neue Materialien, Im Stadtwald, Gebaude 43, D66-123 Saarbrucken, Germany
~Received 16 July 1996; revised manuscript received 15 October 1996!
We report on efficient frequency upconversion in Er31-doped fluoroindate glass. The process is observedunder 1.48mm laser diode excitation and results in fluorescence generation in the range from ultraviolet tonear-infrared radiation. The study was performed for samples containing 1, 2, and 3 ErF3 mol % in the rangeof temperatures from 24 to 448 K. The upconverted signals were studied as a function of the laser intensity,and their dynamical behavior is described using a rate equation model which allows us to obtain the energytransfer rates between Er31 ions in pairs and triads.@S0163-1829~97!07509-7#arbilhe
ereredThe0 KI. INTRODUCTION
In the past years fluoride glasses doped with rare-e~RE! ions have received great attention due to the possities of using these materials in numerous applications sucthe operation of upconversion lasers, superfluorescsources, and optical amplifiers, among others.1 Fluorideglasses are particularly attractive hosts because they cafibered, maintaining a high intensity of pumping light overlong interaction length, and large RE concentrations canincorporated easily into the host matrix. Furthermore, onethe advantages of fluoride hosts is the low energy of its menergetic phonons, which reduces the probability of mtiphonon relaxation processes between the RE electrlevels.
Among the many fluoride compositions discovered, it wfound recently that fluoroindate glasses may become oneportant material for photonics applications. The vitreousgion in the system InF3-ZnF2-~SrF2-BaF2! was establishedfew years ago,2 and it was later observed that the glassesbe stabilized by addition of GaF3, GdF3, CaF2, and NaF.
Previous works performed in this system include the studytheir vibrational spectra and structure4 and the spectroscopof samples doped with Nd31,5 Pr31,5 Eu31,6 and Gd31.6 Ourrecent studies have shown that when doped with Er31, Nd31,and Pr31, the fluoroindate glass presents large efficiencyupconverters from the infrared to visible7 and from orange toblue and violet.8,9
Erbium ions are appealing for spectroscopic investigatdue to their energy level regular spacing which facilitafrequency upconversion via energy transfer or multispump absorption using a single excitation wavelength. Acordingly, studies of upconversion in Er31-doped fluoride,10
borate,11 tellurite and gallate,12 and fluorophosphate glasses13
have been reported. Presently, it is well known that theconversion efficiency is larger for fluoride glasses becathe multiphonon emission rates are much lower than the rfor the same levels of Er31 in other glasses.1,14550163-1829/97/55~10!/6335~8!/$10.00thi-asnt
In the present work we report results of our investigatioon the upconversion properties of Er31-doped fluoroindateglass using the infrared radiation from a cw diode laser asexcitation source. This work extends our previous rootemperature studies7 for the whole range of temperaturefrom 24 to 448 K.
II. EXPERIMENTAL DETAILS
The glasses studied have the following % mocomposition: ~392x!InF3-20ZnF2-16BaF2-20SrF2-2GdF3-2NaF-1GaF32xErF3 ~x51,2,3!. The samples preparatioprocedure is briefly described. InF3 was obtained by fluora-tion of In2O3 at 400 C with NH4F and HF in a platinumcrucible. Then all fluoride components were mixed up aheated in a dry box under argon atmosphere at 700 Cmelting and 800 C for finning. After this process the mwas poured and cooled into a preheated brass mold.samples obtained have good optical quality, volumes ofew cubic centimeters, and they are nonhygroscopic.
Optical absorption spectra in the 200800 nm range wobtained with a double-beam spectrophotometer, whileinfrared spectra up to 1.8mm were measured with an opticaspectrum analyzer.
Continuous-wave upconversion fluorescence measments were performed using a diode laser emitting at 1mm as the excitation source. The laser beam was choppe7 Hz and focused on the sample using a lens of 15 cm folength. The sample fluorescence was collected perpendlarly to the direction of the incident beam and was disperby a 0.5-m grating spectrometer. The signal was detecusing either a GaAs or aS1 photomultiplier, and it was sento a lock-in amplifier or a digital oscilloscope connected topersonal computer for processing.
For the low-temperature measurements, the samples wmounted in a cold-finger Dewar with temperature measuby a thermocouple embedded in the mounting bracket.temperature of the samples could be varied from 24 to 306335 1997 The American Physical Society
6336 55MACIEL, de ARAUJO, MESSADDEQ, AND AEGERTERwith regulation of 0.1 K. For the high-temperature expements, the samples were warmed up to 448 K bytemperature-controlled thermal plate with regulation61 K.
III. RESULTS AND DISCUSSION
Figure 1 shows the room-temperature absorption spein the visible range~a! and in the near infrared~b!, obtainedfor one of the samples prepared. The broad features oferal angstroms bandwidth can be identified with the trantions from the ground state~4I 15/2! to the excited states of thEr31 ions. The bands observed at 274 and 256 nm are duelectronic transitions in the Gd31 ions present in the glasmatrix. No changes in the wavelengths of maxima were
FIG. 1. Room-temperature absorbance spectra in the visible~a!and in the near-infrared~b! regions~sample withx53, thickness 2.5mm!.-af
served for the different concentrations used because thetronic transitions within the 4f shell are not very sensitive tothe crystalline field. The spectra obtained for the othsamples are similar, except for the band intensities, whdepend on the Er31 concentration. The linewidths of all transitions are inhomogeneously broadened due to the site-tovariation of the crystalline field strength.
Figure 2 shows the upconversion spectrum of the samwith x53 under 5.6 mW excitation~;170 W/cm2! at roomtemperature. The diode laser excites resonantly4I 15/24I 13/2 transition and the observed emissions corspond to radiative transitions in the erbium ions from texcited states. The distinct emissions correspond to the tsitions2H9/24I 15/2 ~;407 nm!, 2H11/24I 15/2 ~;530 nm!,4S3/24I 15/2 ~;550 nm!, 4F9/24I 15/2 ~;670 nm!,4I 9/24I 15/2 ~;808 and;827 nm!, 4S3/24I 13/2 ~;854 nm!,and4I 11/24I 15/2 ~;980 nm!. The green and red transitionare readily visible by the naked eye. The spectra were alyzed with respect to their pump power dependence and tporal behavior. To analyze the results we first note thatunsaturated frequency upconversion the fluorescence sI S will be proportional to some powern of the excitationintensity such thatI S}I
n, wheren52,3,4, . . . is thenumberof infrared photons absorbed per upconverted photon eted. The dependence of the fluorescence signal on1.48-mm excitation intensity was such that 3.6,n,3.9 forthe emission at 407 nm, 2.4,n,2.7 for the emission at 550and 670 nm, 1.7,n,2.0 for the emission at 808 and 82nm, 2.4,n,3.3 for the emission at 854 nm, and 1.8,n,2.0for the emission at 980 nm. The measurements were mfor the three concentrations prepared, and the data for onthe samples are shown in Fig. 3. From the intensity depdence observed and the wavelength of the emitted radiatiwe conclude that four laser photons are involved in the 1.mmto407-nm conversion, three laser photons participin the 1.48mm-to-550-nm, 1.48-mm-to-670-nm, and 1.48-mm-to-854-nm conversions, and two laser photons prodthe 1.48-mm-to-808-nm, 1.48-mm-to-827-nm, and 1.48-mm-to-980-nm frequency upconversions. The deviation fromexactn values are due to strong absorption at 1.48mm, theabsorption of the upconverted fluorescence, and becausnonradiative decay from higher-lying states to fluorescstates may also contribute to the intensities of the obserspectral lines. The fluorescence line peaked at 980 nmthe most intense, being'50 times more intense than thtransition at 550 nm. For an incident power of 5 mW, abo1 mW is converted into 980 nm emission. We also observthat for the sample withx53 the signal at 980 nm was twiclarger than for the sample withx52 and 12 times larger thanfor the sample withx51.
Different processes may lead to the population of higexcited Er31 states after excitation in the near infrare(4I 15/24I 13/2).13,1519These processes rely either on mulstep excited state absorption~ESA! or energy transfer~ET!between Er31 ion neighbors. The ET process, in which aexcited ion nonradiatively transfers its energy to an alreaexcited neighbor, is one of the most efficient mechanisand has been observed in a large number of systems incing fluoroindate glasses.814 This mechanism can arise fromelectric multipole or exchange interactions, and its ratecurrence depends on the RE concentration due to the ion